Effect of TiO2 nanotubes with TiCl4 treatment on the photoelectrode of dye-sensitized solar cells
© Meen et al.; licensee Springer. 2012
Received: 16 July 2012
Accepted: 9 October 2012
Published: 23 October 2012
In this study, we used the electrochemical anodization to prepare TiO2 nanotube arrays and applied them on the photoelectrode of dye-sensitized solar cells. In the field emission scanning electron microscopy analysis, the lengths of TiO2 nanotube arrays prepared by electrochemical anodization can be obtained with approximately 10 to 30 μm. After titanium tetrachloride (TiCl4) treatment, the walls of TiO2 nanotubes were coated with TiO2 nanoparticles. XRD patterns showed that the oxygen-annealed TiO2 nanotubes have a better anatase phase. The conversion efficiency with different lengths of TiO2 nanotube photoelectrodes is 3.21%, 4.35%, and 4.34% with 10, 20, and 30 μm, respectively. After TiCl4 treatment, the efficiency of TiO2 nanotube photoelectrode for dye-sensitized solar cell can be improved up to 6.58%. In the analysis of electrochemical impedance spectroscopy, the value of Rk (charge transfer resistance related to recombination of electrons) decreases from 26.1 to 17.4 Ω when TiO2 nanotubes were treated with TiCl4. These results indicate that TiO2 nanotubes treated with TiCl4 can increase the surface area of TiO2 nanotubes, resulting in the increase of dye adsorption and have great help for the increase of the conversion efficiency of DSSCs.
KeywordsTiO2 nanotube arrays dye-sensitized solar cells TiCl4 treatment
Dye-sensitized solar cells (DSSCs) have received considerable attention lately because they are cost-effective and environmentally friendly with efficiencies comparable to those of the traditional silicon-based cells. Generally, granular titanium dioxide powder is commonly used in dye-sensitized solar cell light anode structure. The sol–gel method is used to produce porous film structure, but small pores form between particles of the transmission path of clutter, resulting in a more dye adsorption capacity and low clutter of electron transfer path. The path is too long and will make the leakage current and the probability of electron recombination, thus affecting the overall conversion efficiency of solar cells. The titanium dioxide nano-tubular structure of high surface area and large aspect ratio can be beneficial to the dye adsorption, and more rules of order can be reduced when the electron and hole in the transmission probability of recombination. TiO2 nanotubes have been synthesized by various methods including hydrothermal method, seeded growth, template-assisted deposition, and anodization. Especially, anodization is a relatively simple method for synthesizing large-area and self-organized TiO2 nanotube arrays[6–8]. In this paper, we used the electrochemical anodization to prepare TiO2 nanotubes arrays with different thickness and applied them on the photoelectrode of dye-sensitized solar cells. The TiO2 nanotubes and solar cells were investigated by field-emission scanning electron microscopy, X-ray diffraction (XRD), I V characteristic analyses, and electrochemical impedance spectroscopy (EIS) to study the effect of titanium tetrachloride (TiCl4) treatment on the photoelectrode of TiO2 nanotubes for dye sensitized solar cells.
In this study, the growth of nanotubes was anodized on Ti foils (purity of 99.6%, thickness of 0.2 mm) by constant current at 15 mA in the ethylene glycol solution containing 0.3 wt.% NH4F and 2 vol.% deionized water kept at 20°C. The anodized TiO2 nanotubes were annealed in oxygen at 450°C for 60 min. For the treatment of TiCl4, TiO2 nanotubes were immersed in 0.2 M TiCl4 solution for 1 h and annealed in air at 350°C for 30 min. Pt counter electrodes were prepared by coating with a drop of H2PtCl6 solution and heating at 400°C for 15 min. To adsorb N3 dye, TiO2 nanotubes were immersed in 3×10−4 M solution containing N3 dye and ethyl alcohol at 45°C for 8 h in the oven. The working electrodes were then rinsed with ethanol. Electrolyte solution is adopted from Everlight Chemical Industrial Corporation (ESE-20). The electrode was assembled into a sandwich-type open cell using platinum plate as a counter electrode. Both electrodes were spaced by a kind of polymer films. The thickness was 60 μm, and the size of TiO2 working electrode was 0.25 cm2 (0.5 ×0.5 cm). The surface morphology of the TiO2 nanotubes was observed by scanning field emission electron microscopy. Structural analysis was carried out by powder X-ray diffraction (XRD). The ultraviolet–visible absorption spectrum of the TiO2 electrodes was observed by a UV–vis spectrophotometer. The current–voltage characteristics and impedance of samples were measured by Keithley 2400 source meter (Keithley Instruments Inc., Cleveland, OH, USA), and EIS was determined under simulated sunlight with white light intensity, PL = 100 mW/cm2.
Results and discussion
The parameters of current–voltage characteristics for DSSCs with different lengths of TiO 2 nanotubes
The parameters of current–voltage characteristics for DSSCs with different lengths of TiO 2 nanotubes after TiCl 4 treatment
Sample (μm) with TiCl4
The parameters of EIS calculated from Figure 5 for dye-sensitized solar cells with and without TiCl 4 treatment
20 μm without TiCl4
20 μm with TiCl4
In summary, we prepared TiO2 nanotube arrays by electrochemical anodization to apply on the electrode of dye-sensitized solar cell. After TiCl4 treatment, the walls of TiO2 nanotubes were coated with TiO2 nanoparticles. It can increase the surface area of TiO2 and the adsorption of N3 dye, resulting in better transport properties of TiO2 nanotubes and the improvement of conversion efficiency of DSSCs.
Dye-sensitized solar cells
Electrochemical impedance spectroscopy
- I-V characteristics:
- J sc :
Short-circuit current density
- η :
Overall conversion efficiency
- V oc :
Open circuit potential
This research is supported by the National Science Council, R.O.C., under contract nos. NSC 100-2622-E-150-014-CC3 and NSC 100-2221-E-150-058.
- Alivov Y, Fan ZY: Dye-sensitized solar cells using TiO2 nanoparticles transformed from nanotube arrays. J Mater Sci 2010, 45: 2902–2906. 10.1007/s10853-010-4281-2View ArticleGoogle Scholar
- Tsai CC, Teng HS: Regulation of the physical characteristics of titania nanotube aggregates synthesized from hydrothermal treatment. Chem Mater 2004, 16: 4352–4358. 10.1021/cm049643uView ArticleGoogle Scholar
- Tian ZRR, Voigt JA, Liu J, McKenzie B, Xu HF: Large oriented arrays and continuous films of TiO2-based nanotubes. J Am Chem Soc 2003, 125: 12384–12385. 10.1021/ja0369461View ArticleGoogle Scholar
- Sander MS, Cote MJ, Gu W, Kile BM, Tripp CP: Template-assisted fabrication of dense, aligned arrays of titania nanotubes with well-controlled dimensions on substrates. Adv Mater 2004, 16: 2052–2057. 10.1002/adma.200400446View ArticleGoogle Scholar
- Gong D, Grimes CA, Varghese OK, Hu WC, Singh RS, Chen Z, Dickey EC: Titanium oxide nanotube arrays prepared by anodic oxidation. J Mater Res 2001, 16: 3331–3334. 10.1557/JMR.2001.0457View ArticleGoogle Scholar
- Mor GK, Varghese OK, Paulose M, Mukherjee N, Grimes CA: Fabrication of tapered, conical-shaped titania nanotubes. J Mater Res 2003, 18: 2588–2593. 10.1557/JMR.2003.0362View ArticleGoogle Scholar
- Macak JM, Tsuchiya H, Schmuki P: High-aspect-ratio TiO2 nanotubes by anodization of titanium. Angew Chem Int Ed 2005, 44: 2100–2102. 10.1002/anie.200462459View ArticleGoogle Scholar
- Yang Y, Wang X, Li L: Synthesis and growth mechanism of graded TiO2 nanotube arrays by two-step anodization. Materials Science and Engineering B 2008, 149: 58–62. 10.1016/j.mseb.2007.12.006View ArticleGoogle Scholar
- Ito S, Murakami TN, Comte P, Liska P, Grätzel C, Nazeeruddin MK, Grätzel M: Fabrication of thin film dye sensitized solar cells with solar to electric power conversion efficiency over 10%. Thin Solid Films 2008, 516: 4613–4619. 10.1016/j.tsf.2007.05.090View ArticleGoogle Scholar
- Mor GK, Shankar K, Paulose M, Varghese OK, Grimes CA: Use of highly-ordered TiO2 nanotube arrays in dye-sensitized solar cells. Nano Lett 2006, 6: 215–218. 10.1021/nl052099jView ArticleGoogle Scholar
- Roy P, Kim D, Lee K, Spiecker E, Schmuki P: TiO2 nanotubes and their application in dye-sensitized solar cells. Nanoscale 2010, 2: 45–59. 10.1039/b9nr00131jView ArticleGoogle Scholar
- Ho SY, Su C, Cheng CC, Kathirvel S, Li CY, Li WR: Preparation, characterization, and application of titanium nano-tube array in dye-sensitized solar cells. Nanoscale Res Lett 2012, 7: 147. 10.1186/1556-276X-7-147View ArticleGoogle Scholar
- Kern R, Sastrawan R, Ferber J, Stangl R, Luther J: Modeling and interpretation of electrical impedance spectra of dye solar cells operated under open-circuit conditions. Electrochim Acta 2002, 47: 4213–4225. 10.1016/S0013-4686(02)00444-9View ArticleGoogle Scholar
- Han L, Koide N, Chiba Y, Islam A, Mitate T: Modeling of an equivalent circuit for dye-sensitized solar cells: improvement of efficiency of dye-sensitized solar cells by reducing internal resistance. Comptes Rendus Chimie 2006, 9: 645–651. 10.1016/j.crci.2005.02.046View ArticleGoogle Scholar
- Adachi M, Sakamoto M, Jiu J, Ogata Y, Isoda S: Determination of parameters of electron transport in dye-sensitized solar cells using electrochemical impedance spectroscopy. J Phys Chem B 2006, 110: 13872–13880. 10.1021/jp061693uView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.